CIVIL ENGINEERING Utilization of cement treated recycled concrete aggregates as base or subbase layer in Egypt Ahmed Ebrahim Abu El-Maaty Behiry * Engineering Faculty, Civil Department, Menouﬁa University, Shibeen El-kom City, Egypt Received 13 November 2012; revised 21 January 2013; accepted 14 February 2013 Available online 16 March 2013 KEYWORDS Recycled concrete; Cement treatment; Tensile strength; Compressive strength; Resilient modulus; Base aggregate Abstract Recently, environmental protection has a great concern in Egypt where recycling of increased demolition debris has become a viable option to be incorporated into roads applications. An extensive laboratory program is conducted to study the feasibility of using recycled concrete aggregate (RCA) mixed with traditional limestone aggregate (LSA) which is currently being used in base or subbase applications in Egypt. Moreover, the inﬂuence of mixture variables on the mechanical properties of cement treated recycled aggregate (CTRA) is investigated. Models to pre- dict the compressive and tensile strengths based on mixture parameters are established. The results show that the adding of RCA improves the mechanical properties of the mixture where the uncon- ﬁned compressive strength (UCS) is taken as an important quality indicator. Variables inﬂuencing the UCS such as cement content, curing time, dry density play important roles to determine the per- formance of CTRA. Ó 2013 Ain Shams University. Production and hosting by Elsevier B.V. All rights reserved. 1. Introduction Aggregate is an industrial commodity term for sand, gravel, and crushed rock materials, in their natural or processed state, that are used to provide bulk strength and resistance in con- struction applications. Demolition debris such as crushed con- crete, crushed masonry mortar, and asphalt pavement has been signiﬁcantly recycled since the end of the second world war. However, studies about its physical properties, mechanical behavior, and durability are quite recent. Reclaimed Portland cement concrete is the most abundant and available of the po- tential substitutes for natural aggregate in urban areas, espe- cially in Egypt. Recycling of demolition debris into new construction offers a way to reduce waste disposal loads sent to area landﬁlls and to extend the life of natural resources . Many federal and state highway contracts specify use of recycled materials in highway construction where the rate of this usage is inﬂuenced by the availability, engineering perfor- mance, and by ﬁnancial and other marketplace incentives that encourage the use crushed concrete as recycled aggregate. Re- cently, numerous laboratory studies and ﬁeld trials have shown Abbreviations: CBR, California bearing ratio; CTRA, cement treated recycled aggregate; FS, ﬂexural strength; ITS, indirect tensile strength; LSA, limestone aggregate; MDD, maximum dry density; Mr, resilient modulus; OMC, optimum moisture content; Pdr, plastic deformation ratio; PI, plastic index; RCA, recycled concrete aggregate; UCS, unconﬁned compressive strength. * Mobile: +20 01283961800. E-mail address: [email protected]. Peer review under responsibility of Ain Shams University. Production and hosting by Elsevier Ain Shams Engineering Journal (2013) 4, 661–673 Ain Shams University Ain Shams Engineering Journal www.elsevier.com/locate/asej www.sciencedirect.com 2090-4479 Ó 2013 Ain Shams University. Production and hosting by Elsevier B.V. All rights reserved. http://dx.doi.org/10.1016/j.asej.2013.02.005
Ain Shams Engineering Journal (2013) 4, 661–673
Ain Shams University
Ain Shams Engineering Journal
Utilization of cement treated recycled concrete
aggregates as base or subbase layer in Egypt
Ahmed Ebrahim Abu El-Maaty Behiry *
Engineering Faculty, Civil Department, Menoufia University, Shibeen El-kom City, Egypt
Received 13 November 2012; revised 21 January 2013; accepted 14 February 2013Available online 16 March 2013
Abstract Recently, environmental protection has a great concern in Egypt where recycling of
increased demolition debris has become a viable option to be incorporated into roads applications.
An extensive laboratory program is conducted to study the feasibility of using recycled concrete
aggregate (RCA) mixed with traditional limestone aggregate (LSA) which is currently being used
in base or subbase applications in Egypt. Moreover, the influence of mixture variables on the
mechanical properties of cement treated recycled aggregate (CTRA) is investigated. Models to pre-
dict the compressive and tensile strengths based on mixture parameters are established. The results
show that the adding of RCA improves the mechanical properties of the mixture where the uncon-
fined compressive strength (UCS) is taken as an important quality indicator. Variables influencing
the UCS such as cement content, curing time, dry density play important roles to determine the per-
formance of CTRA.� 2013 Ain Shams University. Production and hosting by Elsevier B.V.
All rights reserved.
Aggregate is an industrial commodity term for sand, gravel,
and crushed rock materials, in their natural or processed state,
ratio; CTRA, cement treated
; ITS, indirect tensile strength;
um dry density; Mr, resilient
tent; Pdr, plastic deformation
d concrete aggregate; UCS,
g by Elsevier
y. Production and hosting by Elsev
that are used to provide bulk strength and resistance in con-struction applications. Demolition debris such as crushed con-crete, crushed masonry mortar, and asphalt pavement has been
significantly recycled since the end of the second world war.However, studies about its physical properties, mechanicalbehavior, and durability are quite recent. Reclaimed Portland
cement concrete is the most abundant and available of the po-tential substitutes for natural aggregate in urban areas, espe-cially in Egypt. Recycling of demolition debris into new
construction offers a way to reduce waste disposal loads sentto area landfills and to extend the life of natural resources. Many federal and state highway contracts specify use ofrecycled materials in highway construction where the rate of
this usage is influenced by the availability, engineering perfor-mance, and by financial and other marketplace incentives thatencourage the use crushed concrete as recycled aggregate. Re-
cently, numerous laboratory studies and field trials have shown
that recycled aggregate can totally or partially replace naturalaggregates in road construction .
Potential saving in cost and time of recycling of construc-
tion and demolition debris has made the use of recycled con-crete aggregate (RCA) an attractive alternative to thehighway engineer. To utilize large volumes of construction
and demolition debris, the minimum standards set by AASH-TO, as well as the local specifications, must be met. Since theserecycled materials may be generated on the job site, the quality
control of these recycled materials may change during thecourse of the project. Therefore, highway engineers maychoose to blend the recycled materials with quarried densegraded aggregate which currently being used in base or sub-
base applications . Although many authors have studiedthe possibility of using RCA in applications, there are a few re-searches on the properties and mechanical behavior of mix-
tures treated with cement when used as road subbases orbase in paving roads because of the following reasons :
– improving the workability of road materials;– increasing the strength of the mixture;– enhancing the durability;
– increasing the load spreading capacity.
Cement treated aggregate is described as a mixture in whicha relatively small amount of cement is used as a binder of
coarse aggregates, and which needs a proper water contentfor both compaction and cement hydration. Generally, cementtreated aggregate as a road base material is produced by using
coarse natural or crushed aggregates and designed as a heavytraffic base or a heavy traffic wearing course. Recently, in or-der to protect the natural resource and reduce the environmen-
tal pollution of solid waste, recycling aggregate has beenconsidered to be used in road bases .
2. Recycled concrete aggregate
When using recycled concrete aggregate as a base or subbasecourse, it is necessary to focus on its gradation, angularity,
soundness, and solubility. Drainable bases require a differentgradation than dense bases because drainable base gradationsmay require additional handling of fines waste to prevent clog-ging. Since the base provides the structure for a roadway, the
soundness of the compacted RCA must be accurately dis-cerned in order to ensure that RCA meets the load-bearingrequirements of the pavement structure initially and in the long
term. The angularity of RCA can increase the effort requiredto compact the granular material to dense base specifications.Some RCA can dissolve in the water passing through the pave-
ment system. This dissolved material will raise the pH of thegroundwater and may possibly affect vegetation within thevicinity of the road. When this water containing dissolved con-crete meets the outside air, the carbon dioxide in the atmo-
sphere will precipitate out calcium carbonate, which canpotentially clog up a drainage system .
3. Problem statement and objective
A lot of old buildings in Egypt are collapsed or replacedyearly. As a result, the demolition and structure processes nat-
urally introduce the problem of recycling materials where
crushed concrete accounts for 60–70% of total debris produc-tion in Egypt. Despite that, there have been scarce studies con-cerned with the mechanical and durability properties of
recycled aggregate used as base or subbase layer in Egypt.The main objective of this research is to better understandthe mechanical behavior of recycled mixtures in order to eval-
uate whether they are feasibly useful as granular material inthe base or subbase layer of road pavement. Moreover, RCAmixtures treated with cement are investigated to evaluate the
improving range in mechanical performance. This study gainsa great importance since landfills, and reclamation sites inEgypt will be exhausted in the near future. If recycled concreteaggregates can be reused as base or subbase materials, it will
greatly alleviate the demand and extend the service life of thedumping facilities. To carry out these objectives, laboratorytests such as compaction proctor test, CBR, plate loading test,
unconfined compressive test, and tensile strength are achieved.Many mechanical properties are obtained such as mixturesdensity, plastic deformation, resilient modulus, unconfined
compressive strength, flexural strength, and indirect tensilestrength. Moreover, this paper reviews the parameters thatinfluence the mechanical properties of cement treated recycled
aggregate (CTRA) such as RCA content, cement content, cur-ing time, mixture dry density, fine material content in aggre-gate, and moisture content. Models to predict the unconfinedand tensile strengths are established based on mixture
4. Literature review
4.1. Unbound recycled concert aggregate
Scientific knowledge on the potential for the use of recycledconcrete aggregates in unbound road applications has ad-vanced considerably. In Egypt and many countries and re-
gions, however, the production of recycled concreteaggregate is much lower than the generation of mixed recycledaggregate obtained from the treatment of mixed rubble. This ismade up of materials of various types, such as concrete, ceram-
ics, asphalt, natural stone, as well as organic impurities (suchas wood, plastic, and paper-cardboard), and inorganic impuri-ties (metal and gypsum) . Vegas et al.  constituted a scien-
tific working document for regulating the use of recycledaggregates obtained from the treatment of mixed rubble in un-bound structural road applications. In the short term, the
intention was to continue this work by investigating the condi-tions of use of recycled aggregates of this type in bound appli-cations with cement and lime, applying stricter criteria withregard to mechanical performance and durability.
Arulrajah et al.  considered a comprehensive laboratoryevaluation of the geotechnical properties of five predominanttypes of construction and demolition (C&D) waste materials.
The C&D materials tested were recycled concrete aggregate(RCA), crushed brick (CB), Waste Rock (WR), Reclaimed as-phalt pavement (RAP), and Fine Recycled Glass (FRG). The
geotechnical assessment included particle size distribution,particle density, water absorption, compaction, Los Angelesabrasion, post-compaction sieve analysis, flakiness index,
hydraulic conductivity, and California bearing ratio (CBR)tests. Shear strength properties of the materials were studiedthrough a series of triaxial tests. In terms of usage in pavement
Utilization of cement treated recycled concrete aggregates as base or subbase layer in Egypt 663
subbases, RCA and WR were found to have geotechnical engi-neering properties equivalent or superior to that of typical nat-ural granular subbase materials. CB at the lower target
moisture contents of 70% of the OMC was also found to meetthe requirements of typical quarry granular subbase materials.The properties of CB, RAP, and FRG, however, may be fur-
ther enhanced with additives or mixed in blends with highquality aggregates to enable their usage in pavement subbases.
Cerni et al.  provided a practical and innovative method
for ranking granular material for pavement design on the basisof a performance-related approach such as permanent defor-mation analysis; on the other, they supported the use of con-struction and demolition materials as a sustainable and cost-
effective alternative to traditional aggregates. Arulrajah et al. investigated the recycled crushed brick when blended withrecycled concrete aggregate and crushed rock for pavement
subbase applications. The research indicates that up to 25%,crushed brick could be safely added to recycled concrete aggre-gate and crushed rock blends in pavement subbase applica-
tions. The repeated load triaxial test results on the blendsindicate that the effects of crushed brick content on themechanical properties in terms of permanent deformation
and resilient modulus of both the recycled concrete aggregateand the crushed rock blends were marginal compared to the ef-fects on dry density and moisture content.
Park  tested the physical and compaction properties of
two different recycled aggregates obtained from a housingredevelopment site (RCA1) and a concrete pavement rehabili-tation project (RCA2). The bulk specific gravity and water
absorption values were 2.53% and 2.54% and 1.43% and1.77% for RCA1 and RCA2, respectively. The optimum mois-ture contents were found to be 9% and 12.8%, and the corre-
sponding dry densities were 2.21 and 1.81 Mg/m3 for RCA1and RCA2, respectively. It was apparent that the optimummoisture content increased with an increase in water absorp-
tion of the aggregates. Arulrajah et al.  achieved a labora-tory investigation into the geotechnical properties of recycledconcrete aggregate (RCA). The Los Angeles abrasion loss testsindicated that the RCA is durable. CBR values were found to
satisfy the local state road authority requirements for subbasematerial. Repeated load triaxial tests established that the RCAwould perform satisfactorily as a pavement subbase material in
the field. The results of the laboratory testing undertaken inthis research indicated that RCA satisfied the criteria for usein pavement subbase applications. Arulrajah et al.  indi-
cated that, at a density ratio of 98% compared to maximumdry density obtained in the modified proctor test and withmoisture contents in the range of 65–90% of the optimummoisture content, most of the recycled C&D materials produce
comparatively smaller permanent strain and greater resilientmodulus than natural commonly used granular subbase mate-rials in pavement subbase applications.
According to Fabiana et al. , the possibility of usingcrushed concrete and demolition debris as subbase coarseaggregate was investigated. CBR experiments were conducted,
and the behavior of the recycled materials was compared withthe behavior of limestone. The results showed that CBR ofcrushed concrete was similar to that of natural aggregate. Con-
versely, demolition debris presented a fairly decrease in itsCBR. Bozyurt et al.  demonstrated that the most commonrecycled construction materials used as unbound base coursein pavement construction are recycled concrete aggregate
(RCA) and recycled asphalt pavement (RAP). This studyinvestigated the mechanical properties of RCA and RAP asunbound base, including the relationships between resilient
modulus (Mr) and composition. The NCHRP model was morereliable in capturing Mr dependency on stress state in RCAand RAP. A multiple linear regression model was developed
to predict the Mr of RCA (R2 = 0.96) and RAP(R2 = 0.97). There was a high degree of correlation betweenthe predicted Mr and the physical properties of RCA
(R2 = 0.89) and RAP (R2 = 0.99).Jimenez et al.  in this article evaluates the behavior and
environmental impact of two recycled aggregates from selectedconstruction and demolition waste (CDW) in field conditions.
For this purpose, one experimental unpaved rural road withtwo sections: the first using a mixed recycled aggregate and arecycled concrete aggregate and the second section consisted
of crushed limestone aggregate as a reference. The results showthat recycled aggregates from selected CDW can be used as analternative to natural aggregates in unpaved rural road con-
struction without risk of environmental impact. This study isimportant for increasing recycling rates and creating a marketfor mixed recycled aggregates in Mediterranean countries such
as Egypt, which has one of the lowest recycling rates.
4.2. Cement treated recycled concrete aggregate
Cement treated materials, which are a family of compactedmix-
tures with granular materials, Portland cement and water, havebeen widely applied as road base/subbase pavements. Since1915, when a pavement was constructed and compacted by
using a mixture of shells, sand, and Portland cement, the mate-rials treated by cement vary from coarse-grained aggregates,recycled aggregates to very fine-grained soils . In practice,note that there are also other stabilizing agents to stabilize road
materials. They are lime, granulated blast furnace slag, pozzol-anas, bitumen, and chemical stabilizers. The literature review ofprevious researches has indicated that coarse-grained materials
with low plasticity index are themost appropriate granulates forcement treatment where the cement treated granular materialshave been used as semirigid base course .
Cement treated aggregate material (CTAM) herein is de-scribed as a mixture in which a relatively small amount of ce-ment is used as a binder of coarse aggregates, and which needs
a proper water content for both compaction and cementhydration. Generally, CTAM as a road base material is pro-duced by using coarse natural or crushed aggregates and de-signed as a heavy traffic base or a heavy traffic wearing
course. Recently, in order to protect the natural resourceand reduce the environmental pollution of solid waste, recy-cling aggregates, such as crushed concrete and crushed ma-
sonry, have been considered to be used in road bases .Hilmi et al.  utilized a traditional base material in roadpavements treated with cement content of 2%, 4%, 8%, and
10% by total weight. They reported that the cement contentwas the most important parameter controlling the design life(fatigue performance) of stabilized layers. It should be stressedthat layer thickness was also important on design life. Mixes
having cement content less than 8% might be used as subbasematerials instead of being used in pavement base.
Agrela et al.  investigated the use of mixed recycled ce-
ment treated aggregates to build the subbase and base layers of
664 A. Ebrahim Abu El-Maaty Behiry
roads. They reported that compared with natural aggregates,mixed recycled aggregates had a low optimal density in themodified proctor test because of the increasing percentage of
masonry particles. A greater amount of water was necessaryto enable optimal compaction of cement treated mixed recy-cled aggregates in road subbases. Cement treated mixed recy-
cled aggregates had a lower workability time, and thus, itmight be useful to apply a setting retardant additive. Cementtreated mixed recycled aggregates exhibited good mechanical
performance in terms of adequate compressive strength, lowdeflections under impact load, and appropriate roughnessvalues.
4.3. Tensile and compressive strength of recycled aggregate
Tensile strength is a very important geotechnical parameter topredict the cracking behavior of pavements, earth dams, and
earth structures using stabilized soils. According to many re-searches, the tensile strength to unconfined compressivestrength ratio was approximately 0.13 for lime stabilized soils.
Kumutha and Vijai  reviewed that both unconfined com-pressive and tensile strengths for the stabilized soil (derivedfrom weathered sandstone) treated with carbide lime and fly
ash. They noticed that both tensile strength and unconfinedcompressive strength increased through curing time (7, 28,90, and 180 days), and the ratio of tensile to compressivestrength increased with long-term curing but with different
5. Experimental program and research approach
This study presents a laboratory investigation aimed to char-acterize the behavior of recycled concrete aggregate com-pared with natural aggregate. The first part of research
studies the mechanical characterization of unbound recyclesbase aggregate as well as traditional limestone aggregate todetermine the optimum mixing ratio. The second part is en-
tirely dedicated to study of the performance of cement trea-ted recycled aggregate where a laboratory test program isdeveloped through traditional geotechnical tests. The flow
chart of the experimental study is presented in Fig. 1. Toachieve the above stated objectives, different parametersare evaluated where each parameter is varied in the follow-ing manner.
(1) Recycled aggregate content in the mixtures: tests aremade at (0.0%, 25%, 50%, 75%, and 100%) RCA.
(2) Cement content: the mixtures are designed by adding(4%, 5%, 6%, and 7%) Portland cement.
(3) Curing time: CTRA samples are tested within compres-
sive test after curing periods of (1, 3, 7, 28 days).(4) Mixture dry density: The effect of dry density variation
due to different moisture contents on the UCS is
evaluated.(5) Moisture content: LSA mixtures are prepared with
moisture content ranged from 6.5% to 11.0%, whileRCA mixtures are prepared with moisture content ran-
ged from 7% to 14.0%.(6) Fine material amount: CTRA samples are prepared with
different fine material amounts (5%, 9%, 12%, and
6.1. Natural aggregate
Limestone aggregate LSA taken from the general Nile com-pany of desert roads is used in this research as granular
layer material. The origin of the limestone aggregates isEL-Suez area, in the northeast Egypt. Fig. 2 illustrates thegrading curves of LSA within the specification limits for
highway works in the Egypt. LSA contains an amount offines about 5% with 19% liquid limit and 14% plasticlimit.
6.2. Recycled concrete aggregate
To produce RCA, Portland cement concrete is broken upand crushed. The major intrinsic material properties that
limit the use of RCA are specific gravity, absorption, sound-ness (resistance to environmental conditions such as chemi-cal and physical weathering), gradation, and contaminant
solubility and the potential for groundwater contamination.The major external factors that limit the use of RCA arecost, state specifications, and environmental regulations .
The grain size distribution for RCA is presented in Fig. 2.The amount of fines in this aggregate reaches to about4.8%.
6.3. Portland cement
Portland cement is used as a treatment material for the granu-lar mixtures. The properties of this cement are given in Table 1.
6.4. Standards requirements for granular mixtures
The base/subbase courses must be made according to a speci-
fied aggregate gradation and requirements to insure adequatestability under repeated loads. Table 2 shows the differentspecifications required according Egyptian code for rural and
7. Experimental work
7.1. Aggregate properties
The physical properties of the used natural and recycled
aggregates are summarized in Table 3. The natural aggre-gates have the highest density value, while crushed concretehas the highest water absorption value. Indeed, the high
amount of adhered mortar attached to RCA particle leadsto a decrease in particle density and an increase in the waterabsorption.
7.2. California bearing ratio
CBR tests are performed on untreated compacted blended
mixtures of RCA and LSA as a measure of granular soilstrength. The mixtures are compacted in the test mold of15.24 cm diameter and 12.7 cm height; moreover, 4.54 kg sur-charge weight was applied.
Traditional limestone aggregate
1. Modified Proctor test 2.CBR test 3. Plate loading test
Sieve analysis Physical properties
1. OMC 2. MDD 3. CBR 4. Mr 5. Pdr
1- cement content (4 , 5 , 6 , 7%) 2- mixture dry density 3- moisture content 6.5-11% for LSA 7– 4% for RCA 4- fine material amount (5 ,9 , 12 , 16% ) 5- curing time (1 , 3 , 7 , 28) days
concrete recycled aggregate (RCA)
Blended mixtures (LAS &RCA)
(0.0 , 25 , 50 , 75 , 100%)
Cement treated aggregateUntreated
1-Plate loading test 2-Compressive UCS test
after (3,7,28 days) 3-Indirect tensile strength after (7,28 days) 4-flexural strength after (7,28 days)
1. MDD 2. Mr 3. Pdr 4.UCS 5. ITS 6.FS
Unconfined compressive strength test
Flexural strength test
Figure 1 Flow chart of the experimental plan.
0.01 0.1 1 10 100Sieve Size (mm)
Figure 2 Grain size distribution for aggregates.
Utilization of cement treated recycled concrete aggregates as base or subbase layer in Egypt 665
7.3. Plate loading test preparation
The test-model basically consists of a square iron box of0.5 · 0.5 · 0.5 m dimensions. The aggregate is spread in five
layers of 10.0 cm thickness in the model and compacted man-ually by cylindrical concrete hummer weighted about 10 kg un-der OMC of each mixture. Then, sand cone test is carried out
on the surface of the final compacted aggregate layer to checkthe relative density and make sure that it greater than 95%according to the standards of highways Egyptian Code. Thesurface of compacted aggregates is leveled; then, the loading
circular steel plate of 16 cm diameter and 2.5 cm thickness is
centered. A contact pressure of 0.5 N/mm2 on asphalt surfacelayer is considered. Using the BISAR-linear elastic program,the vertical stress reaches to the base coarse considering5.0 cm asphalt wearing coarse and 5.0 cm asphalt binder
coarse decreases to 0.35 N/mm2. The deflection under the ver-tical stress allowed to reach almost the maximum value after30 min for each cycle. After that, the total load is released,
and the material is allowed sufficient time to rebound. This cy-cle is repeated three times.
7.3.1. Resilient modulus
The resilient modulus obtained from the plate loading test isbased on the elastic theory. When a rigid plate is put on the
surface of the subgrade soil, the resilient modulus is as follows:
Mr ¼ pð1� l2Þp � a2w
where Mr is the resilient modulus (Mpa); p the uniform ap-plied pressure (Mpa); a the radius of circular plate (mm); wthe deflection corresponding to the third load on the rigid
plate test (mm); and l is the Poisson’s ratio of theaggregate.
7.3.2. Permanent deformation
To utilize current mechanistic–empirical methods of pavementdesign, material properties of the pavement system (pavement
Table 2 Egyptian code standards requirements for aggregate mixtures.
Sieve designation % By weight passing square mesh sieve
Grading A Grading B Grading C Grading D Grading E Grading F
Consistency Liquid limit > 25 and plasticity index > 6
Table 3 Properties of natural and recycled aggregates.
Property RCA Limestone Egyptian standard
Unit weight (kg/m3) 2546 2660 Relative density > 95%
Los Angeles abrasion (%) 33.5 40 50 max
Angle of internal friction (�) 47 23 –
Bulk specific gravity 2.4 3.1 ASTM C-127
Water absorption (%) 2.25 1.05 10 max
Poisson’s ratio 0.25 0.35 –
Plastic index (PI) 3.5 5.0 Max L.L 30% Max P.L 8%
Table 1 Properties of the Portland cement.
Properties Value Chemical properties Value
Specific gravity 3.15 CaO (%) 58.32
Initial setting time (min) 150 SiO2 (%) 26.56
Final setting time (min) 185 MgO (%) 1.12
Volume expansion (mm) 2.0 Fe2O3 (%) 3.89
Compressive strength (MPa) Al2O3 (%) 6.58
2 days 22.0 SO3 (%) 3.32
7 days 38.7 LOI (%) 1.25
28 days 46.8 Specific mass (kg 103/m3) 2.96
Specific surface area (mm2/g) 39.78
666 A. Ebrahim Abu El-Maaty Behiry
layer, base, subbase, and subgrade) are needed to analyze itsresponse to traffic-type loading. Knowledge of material prop-
erties allows for the prediction of stresses and strains devel-oped in the pavement system. For flexible pavement design,the prediction of failure is based on determining the plastic
deformation in base layer. The plastic deformation for blendedbase aggregate mixtures can be obtained from the plate testafter the third loading cycle.
7.4. Unconfined compressive strength
For cement treated mixtures, compressive strength tests
(ASTM C 39) are conducted where the preliminary cementcontent by weight or by volume was selected. The unconfinedcompressive strength (UCS) values for aggregate mixtures areobtained by testing cylindrical specimens of dimensions 150
diameters with 300 mm height (length/diameter ratios of about2.00) using steel molds. The cast specimens are kept in ambient
temperature for 24 h; after that, the samples are wrapped indouble layers of wet burlap where placed in moist environmentfor curing. The average unconfined compressive strength of the
cement treated specimens after 1, 3, 7, and 28-days moisturecuring time is obtained.
7.5. Tensile strength
The tensile strength of cement treated recycled aggregate is al-ways considered as a significant material parameter for design-
ing pavement structures. The reason is because the bottom ofthe treated aggregate layer suffers the tensile stress. In general,flexural beam tests and indirect tensile tests have been em-ployed to evaluate the tensile strength of treated aggregate.
Utilization of cement treated recycled concrete aggregates as base or subbase layer in Egypt 667
7.5.1. Flexural strength
Designers of pavement use a theory based on flexural strength(FS). Therefore, laboratory mix design based on flexuralstrength tests may be required. The flexural strength is ex-
pressed as modulus of rupture where determined by standertest method (ASTM C-78). For measuring flexural strength,normal standard size of specimens 150 · 150 · 500 mm is used.
Equal loads are applied at the distance of one-third from bothof the beam supports. As loading increases, if fracture occurswithin the middle one-third of the beam, the maximum tensile
stress reached called ‘‘flexural strength’’ is computed from fol-lowing equation :
FS ¼ pl
L is the beam span between supports; d the depth of beam; bthe width of beam; and p is the rupture load.
7.5.2. Indirect tensile strength
The indirect tensile strength (ASTM C-496) is conducted. Astandard test cylinder specimen (300 · 150 mm diameter) is
placed horizontally between the loading surfaces of compres-sion testing machine. Due to this compressive loading, an ele-ment lying along the vertical diameter is subjected to a vertical
compressive stress which acting for about 1/6 depth. The largerportion of cylinder is subjected to uniform tensile stress actinghorizontally which acting for about 5/6 depth. The indirect
tensile strength (ITS) can be calculated from the following for-mula :
ITS ¼ 2P
L is the length of cylinder; D the diameter of cylinder; and p isthe compressive load at failure.
8. Experimental results
8.1. Moisture–density relationship
Modified proctor compaction test (ASTM D698) is conductedon RCA and LSA blended mixtures. The maximum dry den-
sity (MDD) and optimum moisture content (OMC) are illus-trated in Table 4. The natural aggregates have the highestMDD by about 10% and the lowest OMC. Since the gradingof each aggregates is similar, this difference is mainly attrib-
uted to the physical properties of natural aggregates whichhas the highest particle density and is less porous. RCA hashigher water content where can absorb nearly twice the
amount of water compared with natural aggregate. Thisabsorption can minimize water infiltration into and underhighways that use RCA as road base material. This results
agree with many researches [3,10,12].
Table 4 Compaction test result for untreated mixtures.
Blended name Materials Optimum moistu
Mix RA0 100% LSA 11.0
Mix RA25 75% LSA+ 25% RCA 9.5
Mix RA50 50% LSA+ 50% RCA 10.6
Mix RA75 25% LSA+ 75% RCA 12.3
Mix RA100 100% RCA 14.7
8.2. California bearing ratio
CBR test is carried out in both unsoaked and 4-day soakedconditions where the results are summarized in Fig. 3. Accord-ing to the highway Egyptian standards, the minimum CBR
values for subbase and base courses are 25% and 50%, respec-tively. In unsoaked case, the LSA has the highest CBR value(85%) where the CBR value gradually decreases as the RCAcontent increases. One possible reason is the lower intrinsic
particle strength of RCA which lead to a decrease in the over-all bearing strength of the base or subbase materials. Further-more, it can be seen from Fig. 3 that the influence of the 4-day
soaked period is negligible on the CBR values. The resultproves that the soaked CBR values for all recycled granularaggregate mixtures are greater than 30% where the recorded
swells are less than 0.15% which can be considered negligible.
8.3. Plate loading test results
In the first load cycle, the cumulative deformation increasesrapidly with increasing the vertical pressure. When the totalload releases and the material takes a sufficient time to re-bound, one part of vertical deflection is return and the residual
part is remained as shown in Fig. 4 for limestone aggregatewhich considered as an example for the plate loading test re-sults. The resilient modulus can be calculated after the third
loading cycle from Eq. (1), where the uniform applied pressure(P) equals 0.35 N/mm2 and the radius of circular plate (a)equals 80 mm. As obtained in Table 5, the RCA has high resil-
ient modulus more than LSA where with increasing the RCAcontent in the blended mixtures, Mr values increase. The opti-mal mixing ratio according to Mr is 75% RCA + 25% LSA.
Plastic deformation is related to the stiffness properties of
the material that affect the fatigue cracking of overlying as-phalt layers, whereas the gradual accumulation of permanentdeformations, although very small during each loading cycle,
could lead to the collapse of the structure due to excessive rut-ting. Therefore, the conventional road pavement design ap-proach is based on providing adequate thickness of layers in
such a way that the pavement structure does not experienceshear failure and that unacceptable permanent deformationsoccur in each layer. On the basis of this evidence, an appropri-
ate understanding and characterization of plastic deformationbehavior of granular materials is needed in order to perform asuccessful pavement design . Table 5 shows the total defor-mations as well as the plastic deformation ratios (Pdr) that
means the accumulated plastic deformation divided on the to-tal deformation after the third loading cycle. In fact, the 100%RCA sample donates minimal Pdr (45.5%). The addition of
LSA to the RCA samples aides in increasing the amount ofplastic deformation.
re content (OMC) (%) Maximum dry density (MDD) (t/m3)
85 8279 77
70 67 66 6662 62
Mix RA0 Mix RA25 Mix RA50 Mix RA75 MixRA100
Figure 3 CBR test result for blended granular mixtures.
Figure 4 Cyclic loading test for limestone aggregate.
Table 5 Plate loading test results for granular blended
Blended name Total
Mix RA0 1.12 74.0 34.5
Mix RA25 1.08 66.5 39.3
Mix RA50 0.92 53.7 43.5
Mix RA75 0.82 48.3 49.5
Mix RA100 0.88 45.5 46.8
668 A. Ebrahim Abu El-Maaty Behiry
9. Cement treatment for coarse aggregate
The proportioning design method of cement treated recycled
base aggregate CTRA mixture that applied in the last decadesis tentative. Therefore, the problem of designing a CTRA mix-ture is the lack of an effective procedure that allows predicting
its mechanical properties from mixture parameters like the mixcomposition and the characteristics of components . Thispaper herein studies the influence of mixture variables on themechanical properties of CTRA. The objective is to indicate
the possibility for establishing an effective approach to predictthe mechanical properties on basis of mixture parameters.Selecting the range of the preliminary cement content by
weight or by volume, which is generally determined by the
material type, is investigated by many studies as for exampleArulrajah et al.  as shown in Table 6. According to the nat-ural and recycled aggregate classification in this research, the
cement is chosen to be added by 5% by the mass.Coarse aggregates applied for treated granular layer should
have some basic requirements such as a continuous grading, a
coarse aggregate size and a good aggregate strength. The valueof PI is also considered to determine whether or not the mate-rial is suitable for cement treatment. If the PI is high, the mor-
tar will be soft and slippery under wet conditions. This couldresults in looseness of coarse particles which in turn may resultin raveling .
9.1. Resilient modulus and plastic deformation for mixtures
The blended recycled aggregate mixtures are tested under plateloading test to obtain the resilient modulus and plastic defor-
mation ratio Fig. 5 illustrates a valuable improvement in Mrvalues due to cement treatment where it shows that theimprovement percentage (IV) increases as the RCA increases.
The treated MixRA75 achieved the maximum Mr with IVreaches to 35%. The IV values due to decreasing the plasticdeformation ratio Pdr are illustrated in Fig. 6. It clearly noted
that the cement treatment leads to a great decreasing in plasticdeformation where the maximum decreasing ratio (60.0%) isobtained at MixRA100. The cement treatment advantages inincreasing the resilient modulus or decreasing the plastic defor-
mation are clearly appeared at higher recycles aggregate add-ing content to natural aggregate.
9.2. Unconfined compressive strength
The UCS is generally acknowledged as an important indicatorof the mixture quality of treated aggregate. A number of mix-
ture variables influence its compressive strength are investi-gated such as the cement content, mixture dry density,moisture content, fine materials amount, and curing time.
9.2.1. Influence of cement content
Fig. 7 shows the influence of cement content on the UCS for
LSA as well as RCA after 3 days curing period. A linear rela-tionship may be given to approximate the relationship betweenthe UCS and the cement content. It is clearly noted that RCA
is more sensitive to the change in the cement content where ithas a sharp curve more than LSA. This may be indicates thatthe UCS of concrete recycled aggregate treated with cement isobviously improved with increasing cement content. This crys-
tallizes the importance of RCA usage as treated base course inimproving its compressive strength compared with LSA, espe-cially at higher cement content.
9.2.2. Influence of mixture dry density
The effect of the dry density after compaction due to differentmoisture contents on the UCS after 3 days curing period andcement content of 5% has been studied for both treated LSA
and RCA and illustrated in Figs. 8 and 9. It has been foundthat the UCS increases with the increase in the dry densitywhere the relation is basically linear and may therefore be ex-pressed as a law:
UCS ¼ Kþ nðDÞ ð4Þ
Table 6 Cement requirements for different soil groups .
AASHTO group A-1-a A-1-b A-2 A-3 A-4 A-5 A-6 A-7
Cement by mass (%) 3–5 5–8 5–9 7–11 7–12 8–13 9–15 10–16
Figure 5 Resilient modulus results for RCA blended mixtures.
Mix RA0 Mix RA25 Mix RA50 Mix RA75 Mix RA100
untreated cement treated
IV = 41.0%IV = 36.5%
IV = 44.7% IV = 52.0% IV = 60.0%
Figure 6 Plastic deformation results for RCA blended mixtures.
0 1 2 3 4 5 6 7 8cement content (%)
Figure 7 Influence of the cement content on the UCS.
Utilization of cement treated recycled concrete aggregates as base or subbase layer in Egypt 669
where D is dry density (kg/m3); K is a constant; n is a dimen-sionless constant representing the tangent of the slop angle. Inpractice, the mixture density strongly depends on the degree of
compaction where with the increase in the density, the UCS in-creases. That is one of the reasons that the UCS of treated nat-ural aggregate is achieved by a high degree of compactioncompared to recycled treated aggregate CTRA. As shown in
Figs 8 and 9, the slop of the curve (n) is a function of the mois-ture where decreases with the increase in the moisture contentfor both LSA and RCA. Values of n for RCA are obviously
higher than them for LSA.Moreover, the effect mixing ratio between cement treated
natural and recycled aggregates has been investigated. As
shown in Table 7, the UCS increases and the density decreaseswith the increase in the RCA content. As reported in otherstudies [4,10,18], the lower density observed with increasingrecycled aggregate content does not greatly affect the mechan-
ical behavior of materials treated with cement. The maximumUCS value is obtained at MixRA75 where the natural lime-stone aggregates MixRA0 shows only about 68% compressive
strength after 3 days when compared to the concrete recycledaggregate MixRA100. This percent increases to 77% and90% with increasing the curing periods to 7 and 28 days,
respectively. Based on the previous results, it can be said that
although the low density may be compensated by increasingthe RCA content, it is generally more economic to achieve high
strength by a good compaction.
9.2.3. Influence of moisture content
In order to explore the influence of the moisture content, thedata in Figs. 8 and 9 are represented in Fig. 10. From theregression equations, the multiple R2 for treated recycled
aggregate with moisture content from 7.0% to 9.0% and trea-ted limestone aggregate with moisture content from 6.5% to11.0% are high. However, note that there is a big scatter for
the regression equation of treated RCA when its moisture con-tent ranges from 9.0% to 14% (R2 = 0.7909).
9.2.4. Influence of fine material amount
The linear relationship shown in Fig. 7 is valid for one specificgradation. It means that other physical properties are not con-
sidered, such as aggregate strength and gradation [12,18].Fig. 11 shows the influence the fines content (of grain size be-low 0.075 mm) for both treated RCA and LSA after 3 dayscuring period. It is generally observed that the approximate
strength increases with increasing the cement content. RCAgets higher UCS more than LSA for each fine percent. Itmeans that the linear slope between the UCS and the cement
content is determined by the aggregate type and also the finescontent. The computer program (Datafit9.0) is used for deter-mining the unconfined compressive strength as a function in
cement and fine contents. The following nonlinear relationshipcan be achieved:
UCS ¼ a� Fb � Cc ð5Þ
where UCS is unconfined compressive strength (Mpa); F ispercent of fine content (%); and C is percent of cement content
(%). The coefficients for traditional lime stone aggregate are(a= 0.066, b = 0.466, and c= 1.387 with R2 = 0.932), whilethe coefficients for cement treated recycled aggregate are(a= 0.1257, b = 0.239, and c= 1.486 with R2 = 0.90).
1.4 1.5 1.6 1.7 1.8 1.9 2 2.1
14.0% WC12.0% WC9.0% WC7.0% WC
Wc (%) n7.0 6.5 9.0 3.6512.0 1.7514.0 1.35
dry density (t/m3)
Figure 9 Relations between the UCS and the dry density for treated RCA.
1 1.2 1.4 1.6 1.8 2 2.2 2.4 2.6
Wc (%) n6.5 1.23 8.0 0.789.5 0.56511.0 0.45
dry density (t/m3)
Figure 8 Relations between the UCS and the dry density for treated LSA.
Table 7 Relations between the UCS and the dry density for treated blended mixtures.
Blended treated Mix Density 103 (kg/m3) UCS 3 days (N/mm2) UCS 7 days (N/mm2) UCS 28 days (N/mm2)
Mix RA0 2.43 1.57 1.968 3.138
Mix RA25 2.32 2.46 2.46 3.32
Mix RA50 2.21 3.18 3.54 3.94
Mix RA75 2.08 3.40 3.65 4.12
Mix RA100 1.98 2.29 2.576 3.481
670 A. Ebrahim Abu El-Maaty Behiry
9.2.5. Influence of curing time
The curing age is another important factor affecting the UCS.The UCS development with the curing time at cement content5% and fine amount 5% is shown in Fig. 12. It can be notedthat the UCS approximately increases linearly with the curing
time. A number of researches have reported its influence on theUCS [7,13,15]. For example, the relationship between the UCSand the curing time can be given as following Eq. (6) :
fcðtÞ ¼ fcðtoÞ þ k � log t
where fc(t) is the UCS at curing age of t days and fc(to) is theUCS at curing age of to days. Another adopted prediction
model based on experimental data considering the influenceof the curing time is as shown in following Eq. (7)  wherethis model brings two adjustable variables (a and b) for the
fcðtÞ ¼ fcð28Þt
aþ b � t ð7Þ
where fc(t) is the UCS at time t and fc(28) is the 28-day UCS.Herein, the relationship between the UCS and the curing time
LSA RCA LSA RCA LSA RCA LSA RCA
cement 4% cement 5% cement 6% cement 7%
5% fine9% fine12% fine16% fine
Figure 11 Influence of the fine material amount on UCS.
y = -1.0235x2 + 4.9148x - 4.4035R2 = 0.9058
y = -0.0197x2 + 1.6423x - 0.7558R2 = 0.7909
y = -3.9972x2 + 18.572x - 18.538R2 = 0.9494
0 0.5 1 1.5 2 2.5 3
LSARCA 9-14% WCRCA 7-9% WC
dry density (t/m3)
Figure 10 Influence of the moisture content on the UCS.
1 4 7 10 13 16 19 22 25 28 31curing days
Figure 12 Influence of the curing time on the UCS.
Utilization of cement treated recycled concrete aggregates as base or subbase layer in Egypt 671
is illustrated in the following Eq. (8) where this model bringsthree adjustable variables (a, b and c). The coefficients for tra-ditional limestone aggregate are a = 1.01, b = 1.011, andc = 0.33 with R2 = 0.99, while the coefficients for cement
treated recycled aggregate are a= 1.236, b= 1.068, andc = 0.247 with R2 = 0.95.
UCSðtÞ ¼ a� ðbÞUCSð28Þ � ðtÞc ð8Þ
where UCS(t) is the unconfined compressive strength (Mpa)after curing time t (day).
9.3. Tensile strength results
9.3.1. Flexural strength
For flexural strength, which is an important material parame-ter when designing pavement where it has been shown from
previous literatures that the flexural strength (FS) of CTRAare about 10–20% of the UCS . Fig. 13 illustrates the relationbetweenUCS andFS considering fine amount of (5%, 9%, 12%
and 16%) for both 5%cement treatedLSAandRCAafter 7 and28 days curing period. From results, it can be noted that with theincrease in fine content, the ratio of FS to the UCS increases
within limits from 10% to 20%. This implies that the materialskeleton influences the flexural strength. Furthermore, ForLSA, the ratio of FS/UCS is larger (up to 20%) than it for
Figure 13 Flexural strength plotted against the UCS.
672 A. Ebrahim Abu El-Maaty Behiry
RCA (down to 10%) where the recycled aggregate shows about75–80% of the strength of natural aggregates. On the other
hand, the curing period has no obvious effect on the ratio ofFS/UCS. An approximate relationship between FS and UCScan be given by following Eq. (9) where the coefficients for
LSA are (a = 0.26 and b = 0.271 with R2 = 0.92) while forRCA are (a = 0.24 and b= 0.428 with R2 = 0.93):
FS ¼ aðUCSÞ � b ð9Þ
If the fine amount (F) is considered, the relation can be ex-
pressed as following Eq. (10), where the coefficients for LSAare (a = �0.128, b = 0.154, and c= 2.0 with R2 = 0.983)while for RCA are (a= �0.404, b = 0.28 and c= 0.019 withR2 = 0.96).
FS ¼ aþ b� ðUCSÞ þ c� ðFÞ ð10Þ
Considering these test results shown in Table 8, it isremarkable that with increasing the recycled aggregate contentor decreasing the curing period, the flexural strength as well as
the ratio (FS/UCS) obviously decreases.
9.3.2. Indirect tensile strength
The indirect tensile strength (ITS) is calculated according toEq. (3) for blended granular mixtures treated with 5% cement.As shown in Table 8, concrete recycled aggregate shows only
about 70% strength when compared to natural limestoneaggregates. Moreover, with increasing the recycled aggregatein the mixture, the ITS decreases.
Most recycled aggregates produced in Egypt contain largeamounts of crushed concrete. Thus, detailed research on theapplication of recycled cement treated aggregates to build
the subbase or base layers of roads is therefore needed. It isfound that the mechanical properties of cement treated mix-tures are influenced and determined by a number of variables,
including cement content, curing time, and fine materialamount. Based on the laboratory test results, the followingconclusions are drawn:
1. With increasing the concrete recycled aggregate to naturallimestone aggregate, the maximum density and CBR values
of untreatedmixtures decrease and the optimummoisture con-tent increase. The soaked CBR values for recycled aggregatelie within Egyptian allowable limits. Moreover, the concreterecycled aggregate mixtures donate minimal plastic deforma-
tion while the maximum resilient modulus is achieved atMixRA75. The cement treatment leads to a valuable improve-ment in the resilient modulus reaches to 35% at MixRA75
and in plastic deformation reaches to 60% at MixRA100.2. A linear relationship can be given to approximate the rela-
tionship between the UCS and the cement content where
the UCS of concrete recycled aggregate is obviously higherthan it for limestone aggregate especially with increasingcement content. The dry density or the degree of compac-
tion is an important factor to determine the UCS of treated
Utilization of cement treated recycled concrete aggregates as base or subbase layer in Egypt 673
aggregate where a linear relation correlates them. The UCS
increases, while the density decreases with the increase inthe RCA content.
3. There exists a threshold moisture content (9%) that criti-
cally influences the UCS development of CTRA. Up to thismoisture content, a strong regression equation is achievedbetween dry density and UCS. Beyond this level a big scatterfor the regression equation is obtained. On the other hand,
the UCS approximately increases linearly with the curingtime for both treated recycled and natural aggregates. Therelationship between them is illustrated with three adjust-
able variables thus it produces more accurate estimation.4. With the increase in fine material amount, the strength ratio
(FS/UCS) increases within limits from10% to 20%. The
LSA obtains strength ratio higher than it for RCA wherethe recycled aggregate shows about 75–80% of the flexuralstrength for natural aggregates and about 70% of the indi-rect tensile strength for natural aggregates. The curing per-
iod has no obvious effect on the strength ratio. Generally,the building demolition debris in the base or subbase layerscan be transformed into useful recycled aggregate through
proper processing for pavement designs.
 Gilpin R, Robinson J, David WM, Helen Hyun. Recycling of
construction debris as aggregate in the Mid-Atlantic Region USA.
Resour Conserv Recycl 2004;42:275–94.
 Jimenez J, Ayuso J, Agrela F. Use of mixed recycled aggregates
with a low embodied energy from non-selected CDW in unpaved
rural roads. Constr Build Mater 2012;34:34–43.
 Thomas B, Walter J, Ali M. Utilization of construction and
demolition debris under traffic-type loading in base and subbase
applications. In: Transportation research board 79th annual
meeting 9–13, Washington, DC; 2000.
 Xuan DX, Houben LJM, Molenaar AAA, Shui ZH. Mechanical
properties of cement-treated aggregate material – a review. Mater
 Van de Ven MFC. Material recycling-general report. In: 2nd
International symposium of treatment and recycling of materials
for transport infrastructure, Paris, France, October 24–26, 2005.
 Forster SW. FHWA views on recycling concrete pavements. In:
Federal highway administration international center for aggre-
gates research 5th annual, symposium, 20–23 April, 1997.
 Vegas I, Ibaez JA, Lisbona A, Faras M. Pre-normative research
on the use of mixed recycled aggregates in unbound road sections.
Constr Build Mater 2011;25:2674–82.
 Arulrajah A, Piratheepan J, Disfani M, Bo M. Geotechnical and
geoenvironmental properties of recycled construction and demolition
materials in pavement subbase applications. ASCE J Mater Civ Eng